In crystallography, crystal structure is a description of ordered arrangement of atoms, ions, or molecules in a crystalline material.^{[1]} Ordered structures occur from intrinsic nature of constituent particles to form symmetric patterns that repeat along the principal directions of threedimensional space in matter.
The smallest group of particles in material that constitutes this repeating pattern is unit cell of the structure. The unit cell completely reflects symmetry and structure of the entire crystal, which is built up by repetitive translation of unit cell along its principal axes. The translation vectors define the nodes of Bravais lattice.
The lengths of principal axes/edges, of unit cell and angles between them are lattice constants, also called lattice parameters or cell parameters. The symmetry properties of crystal are described byconcept of space groups.^{[1]} All possible symmetric arrangements of particles in threedimensional space may be described by 230 space groups.
The crystal structure and symmetry play a critical role in determining many physical properties, such as cleavage, electronic band structure, and optical transparency.
Crystal structure is described in terms of the geometry of arrangement of particles in the unit cells. The unit cell is defined as the smallest repeating unit having the full symmetry of the crystal structure.^{[2]} The geometry of the unit cell is defined as a parallelepiped, providing six lattice parameters taken as the lengths of the cell edges (a, b, c) and the angles between them (α, β, γ). The positions of particles inside the unit cell are described by the fractional coordinates (x_{i}, y_{i}, z_{i}) along the cell edges, measured from a reference point. It is thus only necessary to report the coordinates of a smallest asymmetric subset of particles, called the crystallographic asymmetric unit. The asymmetric unit may be chosen so that it occupies the smallest physical space, which means that not all particles need to be physically located inside the boundaries given by the lattice parameters. All other particles of the unit cell are generated by the symmetry operations that characterize the symmetry of the unit cell. The collection of symmetry operations of the unit cell is expressed formally as the space group of the crystal structure.^{[3]}
Vectors and planes in a crystal lattice are described by the threevalue Miller index notation. This syntax uses the indices h, k, and ℓ as directional parameters.^{[4]}
By definition, the syntax (hkℓ) denotes a plane that intercepts the three points a_{1}/h, a_{2}/k, and a_{3}/ℓ, or some multiple thereof. That is, the Miller indices are proportional to the inverses of the intercepts of the plane with the unit cell (in the basis of the lattice vectors). If one or more of the indices is zero, it means that the planes do not intersect that axis (i.e., the intercept is "at infinity"). A plane containing a coordinate axis is translated so that it no longer contains that axis before its Miller indices are determined. The Miller indices for a plane are integers with no common factors. Negative indices are indicated with horizontal bars, as in (123). In an orthogonal coordinate system for a cubic cell, the Miller indices of a plane are the Cartesian components of a vector normal to the plane.
Considering only (hkℓ) planes intersecting one or more lattice points (the lattice planes), the distance d between adjacent lattice planes is related to the (shortest) reciprocal lattice vector orthogonal to the planes by the formula
The crystallographic directions are geometric lines linking nodes (atoms, ions or molecules) of a crystal. Likewise, the crystallographic planes are geometric planes linking nodes. Some directions and planes have a higher density of nodes. These high density planes have an influence on the behavior of the crystal as follows:^{[1]}
Some directions and planes are defined by symmetry of the crystal system. In monoclinic, trigonal, tetragonal, and hexagonal systems there is one unique axis (sometimes called the principal axis) which has higher rotational symmetry than the other two axes. The basal plane is the plane perpendicular to the principal axis in these crystal systems. For triclinic, orthorhombic, and cubic crystal systems the axis designation is arbitrary and there is no principal axis.
For the special case of simple cubic crystals, the lattice vectors are orthogonal and of equal length (usually denoted a); similarly for the reciprocal lattice. So, in this common case, the Miller indices (ℓmn) and [ℓmn] both simply denote normals/directions in Cartesian coordinates. For cubic crystals with lattice constant a, the spacing d between adjacent (ℓmn) lattice planes is (from above):
Because of the symmetry of cubic crystals, it is possible to change the place and sign of the integers and have equivalent directions and planes:
For facecentered cubic (fcc) and bodycentered cubic (bcc) lattices, the primitive lattice vectors are not orthogonal. However, in these cases the Miller indices are conventionally defined relative to the lattice vectors of the cubic supercell and hence are again simply the Cartesian directions.
The spacing d between adjacent (hkℓ) lattice planes is given by:^{[5]}^{[6]}
The defining property of a crystal is its inherent symmetry. Performing certain symmetry operations on the crystal lattice leaves it unchanged. All crystals have translational symmetry in three directions, but some have other symmetry elements as well. For example, rotating the crystal 180° about a certain axis may result in an atomic configuration that is identical to the original configuration; the crystal has twofold rotational symmetry about this axis. In addition to rotational symmetry, a crystal may have symmetry in the form of mirror planes, and also the socalled compound symmetries, which are a combination of translation and rotation or mirror symmetries. A full classification of a crystal is achieved when all inherent symmetries of the crystal are identified.^{[7]}
Lattice systems are a grouping of crystal structures according to the point groups of their lattice. All crystals fall into one of seven lattice systems. They are related to, but not the same as the seven crystal systems.
Crystal family  Lattice system  Point group (Schönflies notation) 
14 Bravais lattices  

Primitive (P)  Basecentered (S)  Bodycentered (I)  Facecentered (F)  
Triclinic (a)  C_{i} 
aP 

Monoclinic (m)  C_{2h} 
mP 
mS 

Orthorhombic (o)  D_{2h} 
oP 
oS 
oI 
oF  
Tetragonal (t)  D_{4h} 
tP 
tI 

Hexagonal (h)  Rhombohedral  D_{3d} 
hR 

Hexagonal  D_{6h} 
hP 

Cubic (c)  O_{h} 
cP 
cI 
cF 
The most symmetric, the cubic or isometric system, has the symmetry of a cube, that is, it exhibits four threefold rotational axes oriented at 109.5° (the tetrahedral angle) with respect to each other. These threefold axes lie along the body diagonals of the cube. The other six lattice systems, are hexagonal, tetragonal, rhombohedral (often confused with the trigonal crystal system), orthorhombic, monoclinic and triclinic.
Bravais lattices, also referred to as space lattices, describe the geometric arrangement of the lattice points,^{[4]} and therefore the translational symmetry of the crystal. The three dimensions of space afford 14 distinct Bravais lattices describing the translational symmetry. All crystalline materials recognized today, not including quasicrystals, fit in one of these arrangements. The fourteen threedimensional lattices, classified by lattice system, are shown above.
The crystal structure consists of the same group of atoms, the basis, positioned around each and every lattice point. This group of atoms therefore repeats indefinitely in three dimensions according to the arrangement of one of the Bravais lattices. The characteristic rotation and mirror symmetries of the unit cell is described by its crystallographic point group.
A crystal system is a set of point groups in which the point groups themselves and their corresponding space groups are assigned to a lattice system. Of the 32 point groups that exist in three dimensions, most are assigned to only one lattice system, in which case the crystal system and lattice system both have the same name. However, five point groups are assigned to two lattice systems, rhombohedral and hexagonal, because both lattice systems exhibit threefold rotational symmetry. These point groups are assigned to the trigonal crystal system.
Crystal family  Crystal system  Point group / Crystal class  Schönflies  Point symmetry  Order  Abstract group 

triclinic  pedial  C_{1}  enantiomorphic polar  1  trivial  
pinacoidal  C_{i} (S_{2})  centrosymmetric  2  cyclic  
monoclinic  sphenoidal  C_{2}  enantiomorphic polar  2  cyclic  
domatic  C_{s} (C_{1h})  polar  2  cyclic  
prismatic  C_{2h}  centrosymmetric  4  Klein four  
orthorhombic  rhombicdisphenoidal  D_{2} (V)  enantiomorphic  4  Klein four  
rhombicpyramidal  C_{2v}  polar  4  Klein four  
rhombicdipyramidal  D_{2h} (V_{h})  centrosymmetric  8  
tetragonal  tetragonalpyramidal  C_{4}  enantiomorphic polar  4  cyclic  
tetragonaldisphenoidal  S_{4}  noncentrosymmetric  4  cyclic  
tetragonaldipyramidal  C_{4h}  centrosymmetric  8  
tetragonaltrapezohedral  D_{4}  enantiomorphic  8  dihedral  
ditetragonalpyramidal  C_{4v}  polar  8  dihedral  
tetragonalscalenohedral  D_{2d} (V_{d})  noncentrosymmetric  8  dihedral  
ditetragonaldipyramidal  D_{4h}  centrosymmetric  16  
hexagonal  trigonal  trigonalpyramidal  C_{3}  enantiomorphic polar  3  cyclic 
rhombohedral  C_{3i} (S_{6})  centrosymmetric  6  cyclic  
trigonaltrapezohedral  D_{3}  enantiomorphic  6  dihedral  
ditrigonalpyramidal  C_{3v}  polar  6  dihedral  
ditrigonalscalenohedral  D_{3d}  centrosymmetric  12  dihedral  
hexagonal  hexagonalpyramidal  C_{6}  enantiomorphic polar  6  cyclic  
trigonaldipyramidal  C_{3h}  noncentrosymmetric  6  cyclic  
hexagonaldipyramidal  C_{6h}  centrosymmetric  12  
hexagonaltrapezohedral  D_{6}  enantiomorphic  12  dihedral  
dihexagonalpyramidal  C_{6v}  polar  12  dihedral  
ditrigonaldipyramidal  D_{3h}  noncentrosymmetric  12  dihedral  
dihexagonaldipyramidal  D_{6h}  centrosymmetric  24  
cubic  tetartoidal  T  enantiomorphic  12  alternating  
diploidal  T_{h}  centrosymmetric  24  
gyroidal  O  enantiomorphic  24  symmetric  
hextetrahedral  T_{d}  noncentrosymmetric  24  symmetric  
hexoctahedral  O_{h}  centrosymmetric  48 
In total there are seven crystal systems: triclinic, monoclinic, orthorhombic, tetragonal, trigonal, hexagonal, and cubic.
The crystallographic point group or crystal class is the mathematical group comprising the symmetry operations that leave at least one point unmoved and that leave the appearance of the crystal structure unchanged. These symmetry operations include
Rotation axes (proper and improper), reflection planes, and centers of symmetry are collectively called symmetry elements. There are 32 possible crystal classes. Each one can be classified into one of the seven crystal systems.
In addition to the operations of the point group, the space group of the crystal structure contains translational symmetry operations. These include:
There are 230 distinct space groups.
By considering the arrangement of atoms relative to each other, their coordination numbers, interatomic distances, types of bonding, etc., it is possible to form a general view of the structures and alternative ways of visualizing them.^{[9]}
The principles involved can be understood by considering the most efficient way of packing together equalsized spheres and stacking closepacked atomic planes in three dimensions. For example, if plane A lies beneath plane B, there are two possible ways of placing an additional atom on top of layer B. If an additional layer were placed directly over plane A, this would give rise to the following series:
This arrangement of atoms in a crystal structure is known as hexagonal close packing (hcp).
If, however, all three planes are staggered relative to each other and it is not until the fourth layer is positioned directly over plane A that the sequence is repeated, then the following sequence arises:
This type of structural arrangement is known as cubic close packing (ccp).
The unit cell of a ccp arrangement of atoms is the facecentered cubic (fcc) unit cell. This is not immediately obvious as the closely packed layers are parallel to the {111} planes of the fcc unit cell. There are four different orientations of the closepacked layers.
One important characteristic of a crystalline structure is its atomic packing factor (APF). This is calculated by assuming that all the atoms are identical spheres, with a radius large enough that each sphere abuts on the next. The atomic packing factor is the proportion of space filled by these spheres which can be worked out by calculating the total volume of the spheres and dividing by the volume of the cell as follows:
Another important characteristic of a crystalline structure is its coordination number (CN). This is the number of nearest neighbours of a central atom in the structure.
The APFs and CNs of the most common crystal structures are shown below:
Crystal structure  Atomic packing factor  Coordination number (Geometry) 

Diamond cubic  0.34  4 (Tetrahedron) 
Simple cubic  0.52^{[10]}  6 (Octahedron) 
Bodycentered cubic (BCC)  0.68^{[10]}  8 (Cube) 
Facecentered cubic (FCC)  0.74^{[10]}  12 (Cuboctahedron) 
Hexagonal closepacked (HCP)  0.74^{[10]}  12 (Triangular orthobicupola) 
The 74% packing efficiency of the FCC and HCP is the maximum density possible in unit cells constructed of spheres of only one size.
Interstitial sites refer to the empty spaces in between the atoms in the crystal lattice. These spaces can be filled by oppositely charged ions to form multielement structures. They can also be filled by impurity atoms or selfinterstitials to form interstitial defects.
Real crystals feature defects or irregularities in the ideal arrangements described above and it is these defects that critically determine many of the electrical and mechanical properties of real materials.
When one atom substitutes for one of the principal atomic components within the crystal structure, alteration in the electrical and thermal properties of the material may ensue.^{[11]} Impurities may also manifest as electron spin impurities in certain materials. Research on magnetic impurities demonstrates that substantial alteration of certain properties such as specific heat may be affected by small concentrations of an impurity, as for example impurities in semiconducting ferromagnetic alloys may lead to different properties as first predicted in the late 1960s.^{[12]}^{[13]}
Dislocations in a crystal lattice are line defects that are associated with local stress fields. Dislocations allow shear at lower stress than that needed for a perfect crystal structure.^{[14]} The local stress fields result in interactions between the dislocations which then result in strain hardening or cold working.
Grain boundaries are interfaces where crystals of different orientations meet.^{[4]} A grain boundary is a singlephase interface, with crystals on each side of the boundary being identical except in orientation. The term "crystallite boundary" is sometimes, though rarely, used. Grain boundary areas contain those atoms that have been perturbed from their original lattice sites, dislocations, and impurities that have migrated to the lower energy grain boundary.
Treating a grain boundary geometrically as an interface of a single crystal cut into two parts, one of which is rotated, we see that there are five variables required to define a grain boundary. The first two numbers come from the unit vector that specifies a rotation axis. The third number designates the angle of rotation of the grain. The final two numbers specify the plane of the grain boundary (or a unit vector that is normal to this plane).^{[9]}
Grain boundaries disrupt the motion of dislocations through a material, so reducing crystallite size is a common way to improve strength, as described by the Hall–Petch relationship. Since grain boundaries are defects in the crystal structure they tend to decrease the electrical and thermal conductivity of the material. The high interfacial energy and relatively weak bonding in most grain boundaries often makes them preferred sites for the onset of corrosion and for the precipitation of new phases from the solid. They are also important to many of the mechanisms of creep.^{[9]}
Grain boundaries are in general only a few nanometers wide. In common materials, crystallites are large enough that grain boundaries account for a small fraction of the material. However, very small grain sizes are achievable. In nanocrystalline solids, grain boundaries become a significant volume fraction of the material, with profound effects on such properties as diffusion and plasticity. In the limit of small crystallites, as the volume fraction of grain boundaries approaches 100%, the material ceases to have any crystalline character, and thus becomes an amorphous solid.^{[9]}
The difficulty of predicting stable crystal structures based on the knowledge of only the chemical composition has long been a stumbling block on the way to fully computational materials design. Now, with more powerful algorithms and highperformance computing, structures of medium complexity can be predicted using such approaches as evolutionary algorithms, random sampling, or metadynamics.
The crystal structures of simple ionic solids (e.g., NaCl or table salt) have long been rationalized in terms of Pauling's rules, first set out in 1929 by Linus Pauling, referred to by many since as the "father of the chemical bond".^{[15]} Pauling also considered the nature of the interatomic forces in metals, and concluded that about half of the five dorbitals in the transition metals are involved in bonding, with the remaining nonbonding dorbitals being responsible for the magnetic properties. Pauling was therefore able to correlate the number of dorbitals in bond formation with the bond length, as well as with many of the physical properties of the substance. He subsequently introduced the metallic orbital, an extra orbital necessary to permit uninhibited resonance of valence bonds among various electronic structures.^{[16]}
In the resonating valence bond theory, the factors that determine the choice of one from among alternative crystal structures of a metal or intermetallic compound revolve around the energy of resonance of bonds among interatomic positions. It is clear that some modes of resonance would make larger contributions (be more mechanically stable than others), and that in particular a simple ratio of number of bonds to number of positions would be exceptional. The resulting principle is that a special stability is associated with the simplest ratios or "bond numbers": 1⁄2, 1⁄3, 2⁄3, 1⁄4, 3⁄4, etc. The choice of structure and the value of the axial ratio (which determines the relative bond lengths) are thus a result of the effort of an atom to use its valency in the formation of stable bonds with simple fractional bond numbers.^{[17]}^{[18]}
After postulating a direct correlation between electron concentration and crystal structure in betaphase alloys, HumeRothery analyzed the trends in melting points, compressibilities and bond lengths as a function of group number in the periodic table in order to establish a system of valencies of the transition elements in the metallic state. This treatment thus emphasized the increasing bond strength as a function of group number.^{[19]} The operation of directional forces were emphasized in one article on the relation between bond hybrids and the metallic structures. The resulting correlation between electronic and crystalline structures is summarized by a single parameter, the weight of the delectrons per hybridized metallic orbital. The "dweight" calculates out to 0.5, 0.7 and 0.9 for the fcc, hcp and bcc structures respectively. The relationship between delectrons and crystal structure thus becomes apparent.^{[20]}
In crystal structure predictions/simulations, the periodicity is usually applied, since the system is imagined as being unlimited in all directions. Starting from a triclinic structure with no further symmetry property assumed, the system may be driven to show some additional symmetry properties by applying Newton's Second Law on particles in the unit cell and a recently developed dynamical equation for the system period vectors ^{[21]} (lattice parameters including angles), even if the system is subject to external stress.
Polymorphism is the occurrence of multiple crystalline forms of a material. It is found in many crystalline materials including polymers, minerals, and metals. According to Gibbs' rules of phase equilibria, these unique crystalline phases are dependent on intensive variables such as pressure and temperature. Polymorphism is related to allotropy, which refers to elemental solids. The complete morphology of a material is described by polymorphism and other variables such as crystal habit, amorphous fraction or crystallographic defects. Polymorphs have different stabilities and may spontaneously and irreversibly transform from a metastable form (or thermodynamically unstable form) to the stable form at a particular temperature.^{[22]} They also exhibit different melting points, solubilities, and Xray diffraction patterns.
One good example of this is the quartz form of silicon dioxide, or SiO_{2}. In the vast majority of silicates, the Si atom shows tetrahedral coordination by 4 oxygens. All but one of the crystalline forms involve tetrahedral {SiO_{4}} units linked together by shared vertices in different arrangements. In different minerals the tetrahedra show different degrees of networking and polymerization. For example, they occur singly, joined in pairs, in larger finite clusters including rings, in chains, double chains, sheets, and threedimensional frameworks. The minerals are classified into groups based on these structures. In each of the 7 thermodynamically stable crystalline forms or polymorphs of crystalline quartz, only 2 out of 4 of each the edges of the {SiO_{4}} tetrahedra are shared with others, yielding the net chemical formula for silica: SiO_{2}.
Another example is elemental tin (Sn), which is malleable near ambient temperatures but is brittle when cooled. This change in mechanical properties due to existence of its two major allotropes, α and βtin. The two allotropes that are encountered at normal pressure and temperature, αtin and βtin, are more commonly known as gray tin and white tin respectively. Two more allotropes, γ and σ, exist at temperatures above 161 °C and pressures above several GPa.^{[23]} White tin is metallic, and is the stable crystalline form at or above room temperature. Below 13.2 °C, tin exists in the gray form, which has a diamond cubic crystal structure, similar to diamond, silicon or germanium. Gray tin has no metallic properties at all, is a dull gray powdery material, and has few uses, other than a few specialized semiconductor applications.^{[24]} Although the α–β transformation temperature of tin is nominally 13.2 °C, impurities (e.g. Al, Zn, etc.) lower the transition temperature well below 0 °C, and upon addition of Sb or Bi the transformation may not occur at all.^{[25]}
Twenty of the 32 crystal classes are piezoelectric, and crystals belonging to one of these classes (point groups) display piezoelectricity. All piezoelectric classes lack inversion symmetry. Any material develops a dielectric polarization when an electric field is applied, but a substance that has such a natural charge separation even in the absence of a field is called a polar material. Whether or not a material is polar is determined solely by its crystal structure. Only 10 of the 32 point groups are polar. All polar crystals are pyroelectric, so the 10 polar crystal classes are sometimes referred to as the pyroelectric classes.
There are a few crystal structures, notably the perovskite structure, which exhibit ferroelectric behavior. This is analogous to ferromagnetism, in that, in the absence of an electric field during production, the ferroelectric crystal does not exhibit a polarization. Upon the application of an electric field of sufficient magnitude, the crystal becomes permanently polarized. This polarization can be reversed by a sufficiently large countercharge, in the same way that a ferromagnet can be reversed. However, although they are called ferroelectrics, the effect is due to the crystal structure (not the presence of a ferrous metal).
Media related to Crystal structures at Wikimedia Commons
Fundamental aspects of materials science  

Materials science 

Classes of materials  
Analysis methods  
Material characteristics 
Key concepts 
 

Characterisation  
Algorithms  
Software  
Databases  
Journals  
Awards  
Organisation 
 
Seven 3D systems 


Four 2D systems 